investigation of optical coherence ... ... optical coherence tomography optical coherence tomography
Post on 25-May-2020
Embed Size (px)
INVESTIGATION OF OPTICAL COHERENCE TOMOGRAPHY IMAGING IN
NYLON 12 POWDER
Adam Lewis1, Nitesh Katta2, Austin McElroy2, Thomas Milner2, Scott Fish3, Joseph Beaman3
1McKetta Department of Chemical Engineering
2Department of Biomedical Engineering 3Department of Mechanical Engineering
Cockrell School of Engineering, The University of Texas at Austin, Austin, TX 78705
Optical Coherence Tomography (OCT) has shown promise as a new process sensor in
selective laser sintering (SLS) which can yield depth resolved data not attainable with
conventional sensors. However, OCT images of nylon 12 SLS parts and powder contain artifacts,
which have not been previously investigated in literature. These artifacts along with the highly
scattering nature of the SLS parts and powder limit the imaging depth, which decreases the
usefulness of OCT imaging. This study seeks to study the causes of the imaging artifacts and
proposes and investigates methods to improve OCT imaging depth in nylon 12 powder.
Selective Laser Sintering
Selective Laser Sintering (SLS) is one the earliest commercialized additive
manufacturing technologies. SLS has found use in a wide swath of industries including
aerospace and medical devices where, according to a recent report, it accounted for the largest
share of the 3D printed medical devices market in 2016 . This powder bed fusion process is
able to produce parts with strengths comparable to injection-molded parts. A schematic
demonstrating how the SLS process works is shown in Figure 1.
Figure 1. Selective Laser Sintering Schematic 
Solid Freeform Fabrication 2017: Proceedings of the 28th Annual International Solid Freeform Fabrication Symposium – An Additive Manufacturing Conference
During the build process, while maintaining the top layer (typically around 100 microns
thick) of polymer powder about 10°C below its melting point, a laser is used to melt select
portions of the powder. Next, a new layer of powder is spread on top of the previous layer and
the process is repeated until the part is completely formed. It is generally desirable to keep the
entire melted material in a liquid state until the entire part can be cooled down as uniformly as
possible in order to minimize thermal stresses and resulting warpage.
The powders used in the SLS process are typically semicrystalline with nylon 12 being
the most common. As mentioned, the nylon 12 is a powder, melt, and solidified part at various
times in the SLS build process. The crystallinity of the nylon varies in each of these phases as
well. Various researchers have measured crystallinity values in nylon powder with values
ranging from 45-51% –. These crystals are largely melted and portions of the powder
become liquid during the build phase. Then, the nylon solidifies as it recrystallizes during
cooling leaving a crystallinity in the cooled parts of around 21-31% depending on build
Figure 2. Schematic of a semicrystalline polymer spherulite 
The crystals in the solidified part grow spherically outward from the nucleation site and
are known as spherulites. The degree of crystallinity of the parts and the size of such spherulites
are affected by the cooling rate with faster cooling times resulting in a lower degree of
crystallinity and smaller spherulites while slower cooling times result in a higher degree of
crystallinity and larger spherulites . The spherulites are semicrystalline meaning that the
material is composed of both crystalline and amorphous regions as shown in Figure 2.
Despite the applications of SLS in various industries, it is common for SLS part
properties to vary, even amongst different specimen contained within the same build. A desire to
improve consistency of parts has led to an interest in improved process sensing and control in the
SLS process. One of the technologies being investigated as an improved process sensor for SLS
is Optical Coherence Tomography (OCT).
Optical Coherence Tomography
Optical coherence tomography (OCT) is an established medical imaging technique based
on coherence interferometry commonly used in biomedical optics and medicine. In that
application, OCT has the ability to provide real time subsurface visualization of human tissues at
sub 10μm resolution. OCT data can be used to produce cross-sectional and volumetric images
from magnitude and echo time delay data of backscattered radiation. A single OCT scan at a
point on the surface of the sample is known as an A-scan and yields depth information at this
point. A collection of subsequent A-scans is called a B-scan and yields a cross sectional image of
the sample. Subsequent B-scans can be combined to yield a 3D representation of the sample as
shown in Figure 3. The backscattered intensity information is typically presented in the false
color of B-scans and volumetric renderings.
Figure 3. Typical OCT data visualization (Left) A-scan (Middle) B-scan (Right) Volumetric
It is important to remember that each pixel in an A-scan is related to the amount of
backscattered radiation collected at a certain time. This causes a millimeter of water to appear
“thicker” than a millimeter of air in an OCT image because of the different speeds of light
propagation in the different media given by their indices of refraction. This also means that when
light scatters off multiple surfaces before being collected, it appears that the backscattering
occurred lower in the B-scan image than it did physically.
Optical Coherence Tomography in Selective Laser Sintering
Research applying OCT to SLS is sparse. In 2015, Guan et al. reported having used OCT
in SLS parts after being built to look at surface voids, surface roughness, and subsurface voids
within a few layers of the surface . It was recognized that adjacent areas of loose and sintered
powder have different attenuation coefficients, and that the subsurface powder scatters more
strongly than sintered material. Therefore, in subsequent work , Guan et al. found a negative
correlation between the number of pixels above a threshold intensity value in OCT B-scans of
SLS parts and the sintering power used to sinter the part. The correlation was most clear at lower
laser powers and dropped off at higher laser powers. They also identified purposefully under
sintered powder beneath a single sintered layer through examination of the attenuation
coefficient of the OCT signal. In 2016, Lewis et al. boresighted an OCT imaging laser with the
sintering laser on an SLS machine in order to image during the SLS build process . It was
found that various layers could be simultaneously differentiated in the OCT images at low laser
powers, potentially opening the way for interlayer bonding characterization. Additionally, a
common defect known as part curl was able to be identified before causing an SLS build to fail.
Thus, OCT has been investigated as an ex-situ defect detection tool, but the OCT imaging
depth of nylon parts has been found to be limited to a few hundred microns, reducing the
usefulness of OCT in that application. Additionally, OCT has shown promise as an in-situ
process sensor capable of providing subsurface information during the SLS build process, but the
highly scattering nature of the nylon 12 parts and powder is not well understood. Furthering this
understanding is valuable to progress both of the mentioned uses of OCT in SLS and is the aim
of the present work.
Materials and Methods
Nylon Powder and Ethyl Cinnamate
All of the powder imaged in this paper was commercially available, virgin PA650 (nylon
12) from Advanced Laser Materials (ALM). The data sheet provided by ALM gives a particle
size range, D10-D90, of 30 to 100 μm and a mean particle diameter of 55 μm. The melting
temperature is reported at 181°C. Nylon powder was imaged in air as well as ethyl cinnamate.
The ethyl cinnamate had a 99% assay, an index of refraction of 1.558, and was obtained from
Sigma Aldrich .
In this work, two different commercially available Fourier domain, swept source OCT
systems were used which will be referred to as System A and System B.
System A comprised of a commercially available AXSUN swept source laser with details
given in Table 1. The lateral resolution is given by the spot size, which was simulated to be 6μm.
The axial pixel resolution was determined by moving the mirror in the sample arm. Using a
precision micrometer (Z825B Thor Labs Inc.), the mirror interface was moved 1 millimeter to
determine the change in the pixel value. This gave a per pixel movement of 3.75 µm/pixel. The
lateral pixel resolution was determined by imaging a ruler and dividing 4mm by the number of
pixels between the 4mm tick marks and was found to be 16 µm/pixel.
The axial (depth) resolution of OCT System A is defined as the smallest